Enhancing Prediction Accuracy In Sift Theory


 Aubrey Allen
 1 years ago
 Views:
Transcription
1 18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department of Mechanical & Aerospace Engineering, Monash University, Clayton, Australia * Corresponding author Keywords: SIFT, matrix failure, polymer composite, failure prediction 1 Introduction In the conventional laminate theory widely used to predict the strength of fibrereinforced polymer composites, the laminae are treated as homogeneous orthotropic materials. Gosse and Christensen [1] adopted a micromechanical approach which predicts separately the failure of the polymer matrix and fibres 1. They used strain invariants as failure criteria and thus this approach was named as Strain Invariant Failure Theory (SIFT). In the application of SIFT, a microstructure analysis is conducted on a unit cell of the composite material that contains a fibre and surrounding polymeric matrix to determine the relationship between the stressstrain states of the whole cell and its matrix and fibre components. This relationship is then used in a structural analysis to predict matrix or fibre failure. In a linear finite element method, the SIFT analysis could be implemented during post processing the results from a computation based on the conventional laminate theory, by correlating the element stressstrain state with matrix and fibre stressstrain states. This theory has been used by a number of researchers and some success has been reported []. For the matrix failure prediction, Gosse and Christensen proposed that two properties that control damage in the matrix, are the first invariant of the strain tensor, J1, and the second invariant deviator, : J = { } 0. 5 = 0.5 [( 1 ) + ( 1 ) + ( ) ] () 1,, are principal strains. where 1 In principle this micromechanical approach may also predict the interfacial failure between the fibre and matrix. These two strain variants can indicate matrix initial failure due to volume increase (dilational strain) and distortional strains respectively. When either of these reaches its critical value, failure will occur. Note that Equation is essentially Von Mises equivalent strain. This paper aims to demonstrate the accuracy of matrix failure prediction could be increased significantly by enhancing these two failure criteria. Discussion about Polymer Failure Criteria In the following discussion four basic load cases will be considered, namely uniaxial compression, pure inplane shear, uniaxial and biaxial, refer to Figure 1. In most part of this paper, only the initial matrix failure is considered, that is the discussion is restricted to the linear elastic condition. (The application to prediction of matrix ultimate failure will be briefly discussed in Section.4.) The stress and strain states under the four load cases are: Uniaxial compression 1 <0, = =0; 1 = 1 /E<0, = = λ 1 Pure inplane shear 1 >0, = 1, =0; 1 =(1+λ) 1 /E>0, = 1, =0 Uniaxial 1 >0, = =0; 1 = 1 /E>0, = = λ 1 Biaxial 1 = >0, =0; 1 = =(1λ) 1 /E, = λ 1 where 1, and are principal stresses, E is the Young s modulus and λ is the Poison s ratio Fig.1. Four basic load cases considered.1 Uniaxial Compression and Pure Shear Cases In terms of the SIFT theory, the failure criterion based on Equation applies to these two cases.
2 It is well known that the strength of polymer materials could be affected by compressive hydrostatic stress. For those polymer materials, to cover both uniaxial compression and pure shear load cases, a yield criterion such as the DruckerPrager criterion [] would be more suitable than Von Mises criterion. Table 1 provides yield strength data for two typical resin materials used in laminate composites. Table 1. Typical resin material strength data [4] Resin Tensile () Compression () Shear () Type 1 Yield strength E=.6GPa Ultimate λ=0.5 strength Type Yield Strength E=.9GPa λ=0.5 Ultimate strength For the prediction of yield strength, if we generate the critical value of from pure shear data, the measured yield strength in the uniaxial compression case will be higher than the predicted using Equation by 11% and 60% respectively for these two materials. This discrepancy can be removed by applying the parameter DruckerPrager criterion (based on Equation ). + BJ1 = A () where and J1 are calculated using Equations 1 and with the measured failure data from compression and shear tests (Table 1); A and B are two parameters determined from this equation. Failure is predicted when: ' = + BJ1 = A (4) where ' is the revised equivalent strain. Equations (5) and (6) below describe the first invariant of the stress tensor, J1, and the second stress invariant deviator, : J = + (5) { } 0. 5 = 0.5 [( 1 ) + ( 1 ) + ( ) ] (6) Only basic failure criteria that are relatively easy to implement are considered in this study. Note the following relationship: 1+ λ = (7) E 1 λ J1 = J1 (8) E The failure prediction equations can alternatively be expressed using stress variables with full equivalence. For isotropic materials, a stress based failure criterion is more commonly used since it is often easier to use and have clearer physical meaning (e.g. hydrostatic pressure effect shown in DruckerPrager criterion). Alternative equations of Equations () and (4) expressed in stresses are: BJ1 A (9) + = = + BJ1 = ' A (10) For the materials listed in Table 1, A and B values calculated are listed in Table. Table. Parameter A and B values Resin Strain based equation Stress based equation A B A B Type 1.5x10 µ Type 1.6x10 µ Uniaxial and Biaxial Tension Cases Before discussing the uniaxial and biaxial cases, we may consider an extreme case where the polymer is loaded with uniformly distributed tensile stress in all the three axial directions. It is well known that the Von Mises yield criterion is not valid in this situation. A DruckerPrager criterion established using parameters determined from compression and shear load cases would also significantly overpredict the strength in this situation. One commonly adopted approach is to use a maximum tensile stress or strain criterion to handle such tensile dominated load conditions, in conjunction with other criteria such as Von Mises or DruckerPrager to handle other load conditions. In contrast, Equation 1 adopted by Gosse and Christensen contains all the principal strain components in linear combination that indicates the volume increase of the material. Bardenheier [56] provided experimental data from uniaxial and biaxial tests of three types of polymer materials. Analysing these data, it is indicated that under a biaxial tensile load condition, prediction based on Equation 1 would significantly
3 underestimate the material strength, refer to Table. The dilational failure could be more accurately predicted using the critical value of, for example: 0.5 J 1 ' = ( ) (11) This fits more closely to the experimental results. Note that as principal stresses are used, Equation 11 is unaffected by any transformation of coordinates. Table. Data from neat resin biaxial tests [56] and errors with different prediction methods Resin Stress applied* Error with prediction method** (%) 1 Eqn Eqn (11) Max stress criterion Type A Type B Type C * Expressed using the ratio of the yield stress in the biaxial test against that in the uniaxial tensile test ** In each method, the yield stress from the uniaxial tensile test was used to determine the critical value for prediction of yield strength in biaxial tests. A + sign means overprediction and a  sign means underprediction.. Combined Failure Envelope Figure illustrates a failure envelope with the planestress condition ( 0). The portion of the failure envelope formed with the DruckerPrager failure criterion has two parts. The solid line part ( CS ) is established with the uniaxial compression and pure shear test data as discussed in Section.1, whilst the fine dot line part ( ST ) is established with the pure shear and uniaxial tensile data in a similar way. This figure shows that the portion of the failure envelope formed with the DruckerPrager failure criterion can intersect with uniaxial compression, pure shear and uniaxial tensile test data points and join with the J 1 curve smoothly, that indicates significantly improvement. (Regarding the curve smoothness, note that a significant improvement of the VonMises criterion over the maximum shear (Tresca) criterion is that it smooths the curve and removes the singular points in Tresca criterion.) In the dimensional space with 1,, coordinate axes, the failure envelope is represented by two cone surfaces (formed with the DruckerPrager failure criterion, with the axis along the line 1 = = and joined at = 0) truncated by a hemisphere surface (formed with J 1 = the uniaxial tensile yield stress). UC CS J 1 UT ST J 1UT UT = uniaxial tensile; BT = biaxial tensile; PS = pure shear; UC = uniaxial compression; UC = with critical value determined from uniaxial compression test; CS = with parameters determined from uniaxial compression and shear tests; ST = with parameters determined from shear and uniaxial tensile tests; J 1UT = J 1 with critical value determined from uniaxial tensile test; and J 1 UT = J 1 with critical value determined from uniaxial tensile test. Fig.. Illustration of failure envelope (planestress).4 Matrix Ultimate Failure Prediction By using the ultimate strength and secant stiffness to replace yield strength and initial linear stiffness, the above analysis may be extended to cover prediction of matrix ultimate failure with linear analyses. Note that: The accuracy of DruckerPrager criterion over Von Mises failure criterion has been clearly observed particularly for the ultimate strength of many polymer materials; and Use of a linear analysis with secant stiffness to approximate a nonlinear analysis is a widely used analysis method and thus may be significant for practical applications. Lamina Unit Cell Analysis A unit cell analysis using a finite element method was further conducted with the four typical load cases discussed above. The failure prediction based on Equation and Equation () was compared with that based on Equations (10) and (11) when both fibre and matrix are present. 1
4 As the discussion in Section indicated that the failure criteria proposed in this paper could predict neat resin failure more accurately, Equations (10) and (11) are used as a yardstick in this comparison..1 Finite Element Model The following typical material properties are assumed: Fibre Young s modulus (E f ) = 00 GPa Fibre Poisson ratio (λ f ) = 0. Matrix Young s modulus (E m ) =.6 GPa Matrix Poisson ratio (λ m ) = 0.5 Fibre volume fraction (V f ) = 0.5 Referring to Figure, with a relatively low fibre volume fraction of 0.5, a square pattern fibre distribution in the matrix can be assumed (as opposed to a hexagon pattern). A unit cell was extracted with two different orientations. A FEM model is shown in Figure 4. Considering the symmetrical condition, only one eighth of the unit cell was built. remaining unloaded surfaces were given a uniform displacement, that results in the gross load on the surface being zero, to reflect the Poisson effect. The loading and boundary conditions applied ensure all the surfaces are kept straight, as required for simulation of a unit cell in a lamina structure.. Results and Discussion..1 Compression and Shear Load Cases The unit cell shown in Figure (a) was considered. As expected, for the matrix material in the uniaxial compression case, high compressive stress concentration (over 4 times the average strain of the unit cell) occurred at the area indicated in Figure 5(a). Due to the Poisson effect from the stiff fibre, the other two stress components perpendicular to the applied load are also compressive in the high stress concentration area. This results in a relatively high hydrostatic stress in this area and thus the strength predicted with the DruckerPrager type criterion is much higher than that with VonMises criterion. In contrast, in the pureshear case, high compressive and tensile stress concentration occurred separately at the areas shown in Figure 5(b). This results in strength predicted with DruckerPrager type criterion to be much less than that with VonMises criterion in the tensile stress concentration area. Compression stress concentration area Tensile stress concentration area (a) Orientation 1 (b) Orientation Fig.. Unit cells with two orientations (V f = 0.5) (a) (b) Fig.5. Stress concentration areas in uniaxial compression and pure shear load cases Fig.4. A unit cell FEM mesh (oneeighth model of the unit cell in Figure a) The load condition is applied in the form of uniform surface displacement. Symmetry boundary conditions are applied to three orthogonal surfaces. The With a load applied that resulted in 0.01 gross strain, the calculated maximum effective stress values are listed in Table 4. For practical applications of the SIFT approach, the failure strength of the matrix is generally determined using laminate specimen tests rather than from neat 4
5 resin tests [1]. If the strength is calibrated using the uniaxial compression strength for Material Type 1 (Table 1), when predicting strength in the pureshear load case, as indicated in Table 4, the difference between the original SIFT approach and the proposed revised approach is 60.6%. Table 4. Predicted maximum and values under uniaxial compression and pureshear loadings Uniaxial compression () Pureshear Ratio ()/ Discrepancy E.00E %.. Uniaxial and Biaxial Tension Load Cases Figure 6 shows the stress concentration areas in these two load cases for the unit cell shown in Figure (a). In the biaxial case, each of the two stress concentration areas was affected mainly by one of the two loads. Thus there is no significant biaxial tensile stress. Table 5 lists maximum J 1 and J 1 values. Consequently when using the two different methods calibrated using uniaxial tensile state data to predict biaxial state strength, the difference is only.4%. Tensile stress concentration areas (a) (b) Fig.6. Stress concentration areas in uniaxial and biaxial load cases  Orientation 1. The unit cell shown in Figure (b) was subsequently calculated. The maximum critical value locations in the uniaxial tensile load case are at a positions shown in Figure 7 (a), whilst the maximum critical The effect of scale difference between the unit cell and lamina structure is generally not considered in SIFT, refer to [1], whilst this calibration may, to certain degree, take the scale effect into consideration. value locations in the biaxial tensile load case are at b positions shown in Figure 7(b). These maximum critical values listed in Table 6. Table 5. Predicted maximum J 1 and J 1 values under uniaxial and biaxial loadings  Orientation 1 Uniaxial () Biaxial Ratio ()/ Discrepancy J J 1.7E a b a.1e % a b a (a) (b) Fig.7. Stress concentration areas in uniaxial and biaxial load cases  Orientation. As shown in Table 6, when using the two different methods calibrated using uniaxial tensile state data to predict biaxial state strength, the difference is 6.1%, in terms of the maximum critical values in the whole matrix, however, for a specific critical location such as at b locations, the two methods yield significant difference. This might have a complicated effect on determining the correlation between the element stressstrain and matrix and fibre stressstrain states. Table 6. Predicted J 1 and J 1 values at critical points under uniaxial and biaxial loadings  Orientation Point a Point b Max Uniaxial () Biaxial Ratio ()/ J Difference J E.44E. 1.0 % J J 1 1.0E.05E % J J E.05E % 5
6 4 Summary The SIFT failure theory separably predicts fibre and matrix failure in a fibre reinforced composite material. Matrix yield prediction is based on a VonMises strain and first strain invariant criteria. Improvement of the matrix failure criteria for prediction accuracy is discussed and demonstrated in this paper. For two typical resin materials, VonMises yield criterion is unable to fit both yield strength values from uniaxial compression and pureshear tests. When calibrated using the measured shear yield strength, the discrepancy between the predicted and measured uniaxial compression strength is found to be 11% and 60% respectively, whilst using a DruckerPrager criterion these discrepancies could be removed. Use of the critical value of the first invariant strain, when calibrated using the uniaxial tensile yield strength, underpredicts the biaxial tensile strength significantly by over 0% on average, compared with available measurement data of neat resin materials. A revised criterion proposed in this paper could reduce the discrepancy to less than 10%. The proposed failure envelope contains Drucker Prager failure criteria, that intersect with all the uniaxial compression, pure shear and uniaxial tensile test data points, and a revised tensile failure criterion. The areas governed by these criteria join each other smoothly. For a unit cell with a fibre and surrounding matrix from a lamina with 50% fibre volume fraction and typical material properties, a FEM analysis conducted in this study indicates that the difference between the yield strength of the matrix material predicted using VonMises and Drucker Prager type criteria is over 60% in the pure shear load case, when the critical values of these yield criteria are determined in the uniaxial compression load case. The FEM analysis showed that the difference between the yield strength of the matrix material in a unit cell predicted using the first strain variant and the revised criterion reaches 6.1% in the biaxial tensile load case, when the critical values of these yield criteria are determined in the uniaxial tensile load case. By using ultimate strengths and secant stiffness to replace yield strengths and initial linear stiffness, the analysis in this paper may be extended to prediction of matrix ultimate failure using linear analyses. Acknowledgement The authors would like to acknowledge that this paper is outcome of a research project of the Cooperative Research Centre for Advanced Composite Structures (CRCACS). References [1] Gosse JH, Christensen S., Strain invariant failure criteria for polymers in composite materials, AIA A. Paper AIAA/ASME/ASCE/ASC conference, Seattle, WA, United States, 001. [] Li R, Kelly D, and Ness R. Application of a first invariant strain criterion for matrix failure in composite materials. Journal of composite Materials, 00. 7(): [] Drucker D C and Prager W. Solid mechanics and plastic analysis for limit design. Quarterly of Applied Mathematics, 10 () , 195. [4] Fei Y P. Mechanics of fibre reinforced composite. Tongji University Press. Shanghai [5] Bardenheier. Mechanicaches Versagen von Polymerwerkstooen. HanserVerlag [6] Kolling S, Haufe A, Feucht M, and Du Bois P A. A constitutive formulation for polymers subjected to high strain rates. 9 th International LSDyna Users Conference. Michigan, June 46,
Constitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationVI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA
VI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA The term critical tests implies more than just a routine comparison with some convenient data. First, a candidate failure criterion
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationDEFORMATION THEORY OF PLASTICITY
DEFORMATION THEORY OF PLASTICITY ROBERT M. JONES Professor Emeritus of Engineering Science and Mechanics Virginia Polytechnic Institute and State University Blacksburg, Virginia 240610219 Bull Ridge Publishing
More informationSSNV221 Hydrostatic test with a behavior DRUCK_PRAGER linear and parabolic
Titre : SSNV221  Essai hydrostatique avec un comportement[...] Date : 08/08/2011 Page : 1/10 SSNV221 Hydrostatic test with a behavior DRUCK_PRAGER linear and parabolic Summary: The case test proposes
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationME111 Instructor: Peter Pinsky Class #21 November 13, 2000
Toda s Topics ME Instructor: Peter Pinsk Class # November,. Consider two designs of a lug wrench for an automobile: (a) single ended, (b) double ended. The distance between points A and B is in. and the
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationApplication of Three Dimensional Failure Criteria on HighPorosity Chalk
, 56 May 00, Trondheim, Norway Nordic Energy Research Programme Norwegian U. of Science and Technology Application of Three Dimensional Failure Criteria on HighPorosity Chalk Roar Egil Flatebø and Rasmus
More informationCIVL4332 L1 Introduction to Finite Element Method
CIVL L Introduction to Finite Element Method CIVL L Introduction to Finite Element Method by Joe Gattas, Faris Albermani Introduction The FEM is a numerical technique for solving physical problems such
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationANALYSIS OF STRAINS CONCEPT OF STRAIN
ANALYSIS OF STRAINS CONCEPT OF STRAIN Concept of strain : if a bar is subjected to a direct load, and hence a stress the bar will change in length. If the bar has an original length L and changes by an
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationFatigue Algorithm Input
Methods Fatigue Algorithm Input By default, fesafe analyses stress datasets that contain elastic stresses The calculation of elasticplastic stressstrains, where necessary, is performed in fesafe using
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationEffect Of The InSitu Stress Field On Casing Failure *
Effect Of The InSitu Stress Field On Casing Failure * Tang Bo Southwest Petroleum Institute, People's Republic of China Lian Zhanghua Southwest Petroleum Institute, People's Republic of China Abstract
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationStrength of Adhesive Joints: A Parametric Study
Project PAJex1  Report 3 Strength of Adhesive Joints: A Parametric Study W R Broughton, L E Crocker and J M Urquhart July 2001 NPL Materials Centre National Physical Laboratory NPL Report MATC(A)27 July
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationSteady Load Failure Theories
tea Loa Failure Theories Ductile Materials Uniaxial tress/train Fiel MaximumNormaltress MaximumNormaltrain Maximumheartress DistortionEnerg hearenerg Von MisesHenck Octaheralheartress InternalFriction
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationRock Failure. Topics. Compressive Strength Rock Strength from Logs Polyaxial Strength Criteria Anisotropic Rock Strength Tensile Strength
Rock Failure Topics Compressive Strength Rock Strength from Logs Polyaxial Strength Criteria Anisotropic Rock Strength Tensile Strength Key Points 1. When rock fails in compression, the compressive stress
More informationA Critical Planeenergy Model for Multiaxial Fatigue Life Prediction. of Homogeneous and Heterogeneous Materials. Haoyang Wei
A Critical Planeenergy Model for Multiaxial Fatigue Life Prediction of Homogeneous and Heterogeneous Materials by Haoyang Wei A Thesis Presented in Partial Fulfillment of the Requirements for the Degree
More informationTheory of Plasticity. Lecture Notes
Theory of Plasticity Lecture Notes Spring 2012 Contents I Theory of Plasticity 1 1 Mechanical Theory of Plasticity 2 1.1 Field Equations for A Mechanical Theory.................... 2 1.1.1 Straindisplacement
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationA ratedependent HosfordCoulomb model for predicting ductile fracture at high strain rates
EPJ Web of Conferences 94, 01080 (2015) DOI: 10.1051/epjconf/20159401080 c Owned by the authors, published by EDP Sciences, 2015 A ratedependent HosfordCoulomb model for predicting ductile fracture at
More informationPredicting Fatigue Life with ANSYS Workbench
Predicting Fatigue Life with ANSYS Workbench How To Design Products That Meet Their Intended Design Life Requirements Raymond L. Browell, P. E. Product Manager New Technologies ANSYS, Inc. Al Hancq Development
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationWellbore stability analysis in porous carbonate rocks using cap models
Wellbore stability analysis in porous carbonate rocks using cap models L. C. Coelho 1, A. C. Soares 2, N. F. F. Ebecken 1, J. L. D. Alves 1 & L. Landau 1 1 COPPE/Federal University of Rio de Janeiro, Brazil
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationOn MooneyRivlin Constants for Elastomers
th International LSDYNA Users Conference Constitutive Modeling() On Mooneyivlin Constants for Elastomers The Mooneyivlin constitutive equation for rubber is W C I C I 3 3 William W. Feng John O. Hallquist
More informationin Ice Crushing Failure
Yield and Plastic Deformation in Ice Crushing Failure TERRANCE D. RALSTON ABSTRACT Plasticity theory has been widely used to describe the deformation and failure of metals, soils, rocks, and concrete.
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationLIMITATIONS OF THE STANDARD INTERACTION FORMULA FOR BIAXIAL BENDING AS APPLIED TO RECTANGULAR STEEL TUBULAR COLUMNS
LIMITATIONS OF THE STANDARD INTERACTION FORMULA FOR BIAXIAL BENDING AS APPLIED TO RECTANGULAR STEEL TUBULAR COLUMNS Ramon V. Jarquio 1 ABSTRACT The limitations of the standard interaction formula for biaxial
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationProf. B V S Viswanadham, Department of Civil Engineering, IIT Bombay
50 Module 4: Lecture 1 on Stressstrain relationship and Shear strength of soils Contents Stress state, Mohr s circle analysis and Pole, Principal stressspace, Stress pathsin pq space; MohrCoulomb failure
More informationA Constitutive Model for Plastics with Piecewise Linear Yield Surface and Damage
6. LSDYNA Anwenderforum, Frankenthal 2007 Crash II  Schadensmodellierung A Constitutive Model for Plastics with Piecewise Linear Yield Surface and Damage M. Vogler 1, S. Kolling 2, A. Haufe 3 1 Leibniz
More informationEFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS
EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationLecture 8 Viscoelasticity and Deformation
HW#5 Due 2/13 (Friday) Lab #1 Due 2/18 (Next Wednesday) For Friday Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, μ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationChapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review
Chapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review Michael Brünig Abstract The paper summarizes the author s activities in the field of damage mechanics. In this
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationUnified elastoplastic finite difference and its application
Appl. Math. Mech. Engl. Ed., 344, 457 474 013 DOI 10.1007/s1048301316837 c Shanghai University and SpringerVerlag Berlin Heidelberg 013 Applied Mathematics and Mechanics English Edition Unified elastoplastic
More informationCentrifuge Shaking Table Tests and FEM Analyses of RC Pile Foundation and Underground Structure
Centrifuge Shaking Table s and FEM Analyses of RC Pile Foundation and Underground Structure Kenji Yonezawa Obayashi Corporation, Tokyo, Japan. Takuya Anabuki Obayashi Corporation, Tokyo, Japan. Shunichi
More information